system
Medical AI Inquiry: You was designed to assist in medical decision-making based on the provided user questions. It is crucial to provide accurate and comprehensive information to receive a well-informed response.  Labels: OBJECTIVE, METHODS, RESULTS. Meshes: Animals, Biomechanical Phenomena, Female, Goats, Male, Proteins, Tibia, Tissue Engineering, Torsion, Mechanical.
user
Does biomechanical research on tissue engineering bone constructed by deproteinated bone? Context: To study biomechanical changes of newly formed bones 24 weeks after repairing large defects of long bones of goats using heterogeneous deproteinated bone (DPB) prepared by modified methods as an engineering scaffold. According to a fully randomized design, 18 goats were evenly divided into three groups: normal bone control group (Group A), autologous bone group (Group B) and experimental group (Group C). Each goat in Groups B and C were subjected to the periosteum and bone defect at middle-lower part of the right tibia (20% of the whole tibia in length), followed by autologous bone or DPB plus autologous MSCs + rhBMP2 implantation, respectively and semi-ring slot fixation; while goats in Group A did not perform osteotomy. At 24 weeks after surgery, biomechanical tests were carried out on the tibias. At 24 weeks after surgery, the results of anti-compression test on tibias in three groups were recorded by a functional recorder presented as linear pressure-deformation curve. The shapes of the curves and their change tendency were similar among three groups. The ultimate pressure values were 10.74 MPa+/-1.23 MPa, 10.11 MPa+/-1.35 MPa and 10.22 MPa+/-1.32 MPa and fracture compression rates were 26.82%+/-0.87%, 27.17%+/-0.75% and 28.22%+/-1.12% in Groups A, B and C, respectively. Comparisons of anti-compression ultimate pressures and fracture compression rates among three groups demonstrated no significant difference (P(AB) equal to 0.415, P(BC) equal to 0.494). Three-point anti-bend test on tibias was recorded as load-deformation curves, and the shapes of the curves and their change tendency were similar among three groups. The ultimate pressure values of the anti-bend test were 481.52 N+/-12.45 N, 478.34 N+/-14.68 N and 475.62 N+/-13.41 N and the fracture bend rates were 2.62 mm+/-0.12 mm, 2.61 mm+/-0.15 mm and 2.81 mm+/-0.13 mm in Groups A, B and C, respectively. There was no significant difference between groups (P(AB) equal to 0.7, P(BC) equal to 0.448). The ultimate anti-torsion torque values were 6.55 Nm+/-0.25 Nm, 6.34 Nm+/-0.18 Nm and 6.42 Nm+/-0.21 Nm and fracture torsion rates were 29.51 degree+/-1.64degree, 28.88 degree+/-1.46 degree and 28.81 degree+/-1.33 degree in Groups A, B and C, respectively. There was no significant difference between groups (P(AB) equal to 0.123, P(BC) equal to 0.346).
assistant
The biomechanical characteristics of newly formed bones from heterogeneous DPB for repairing large segmental long bone defect are comparable to those of normal bones and autologous bones. DPB has the potential for clinical usage as bone graft material. Final Decision: yes